Influence of argon plasma on the deposition of Al2O3 film onto the PET surfaces by atomic layer deposition
© Edy et al.; licensee Springer. 2013
Received: 16 November 2012
Accepted: 4 January 2013
Published: 15 February 2013
In this paper, polyethyleneterephthalate (PET) films with and without plasma pretreatment were modified by atomic layer deposition (ALD) and plasma-assisted atomic layer deposition (PA-ALD). It demonstrates that the Al2O3 films are successfully deposited onto the surface of PET films. The cracks formed on the deposited Al2O3 films in the ALD, plasma pretreated ALD, and PA-ALD were attributed to the energetic ion bombardment in plasmas. The surface wettability in terms of water contact angle shows that the deposited Al2O3 layer can enhance the wetting property of modified PET surface. Further characterizations of the Al2O3 films suggest that the elevated density of hydroxyl -OH group improve the initial growth of ALD deposition. Chemical composition of the Al2O3-coated PET film was characterized by X-ray photoelectron spectroscopy, which shows that the content of C 1s reduces with the growing of O 1s in the Al2O3-coated PET films, and the introduction of plasma in the ALD process helps the normal growth of Al2O3 on PET in PA-ALD.
KeywordsAtomic layer deposition PET film Al2O3 coating
Atomic layer deposition (ALD) is an ultrathin film deposition method by sequential exposure of gas phase reactants for the deposition of thin films with atomic layer accuracy [1–3]. Each atomic layer formed in the sequential process is a result of saturated surface controlled chemical reactions [4–6]. In plasma-assisted atomic layer deposition (PA-ALD), additional energy for the chemical reaction is provided by applying plasmas at an appropriate time interval during the reaction cycle, in which the plasmas are used to produce radicals by gas dissociation [4, 7, 8]. It brings the advantages of improving the reaction rates, the process efficiency, the fragmentation of precursor molecules, and the removal of product molecules [4, 9]. The reactive surface groups play an important role for the initial growth and nucleation of Al2O3 thin film in atomic layer deposition by reacting with the precursor molecules [10–13]. Hydroxyl groups are considered to be the typical reactive groups, which secure a good adhesion of chemical bonding between the underlying substrate and the deposited thin film [5, 13]. The ALD growth of Al2O3 on several polymers with and without reactive surface groups have been investigated with the precursors trimethylaluminum (TMA) and H2O [1, 11, 13], which demonstrated that the initial nucleation on polymers without the reactive surface groups were started by the strong absorption and retention of TMA in the surface layers of polymer, which reacted with the water vapor during the subsequent deposition pulse [11–13]. It suggests that the quality of deposited film depends on the surface coverage in the adsorption step, which is governed by the concentration and spatial distribution of reactive groups on the substrate [5, 14]. It takes 10 to 20 ALD cycles to form the Al2O3 film on the polymer surface before the deposition achieves a normal ALD growth with the deposition rate similar to that observed in the other surfaces . Unfortunately, the understanding of deposition dynamics in ALD by introducing the plasmas is incomplete. Here, studies on ALD and PA-ALD deposition on PET films with and without plasma pretreatment are carried out to demonstrate the influence of argon plasmas on the deposition of Al2O3 film.
Polyethylene terephthalate (PET) film and silicon were used as the substrates. PET is a semi-crystalline polymer at room temperature, which is cleaned by an ultrasonic machine for 20 min with ultrasonic power and temperature of 80 W and 30°C, respectively. The films were dried in a vacuum oven for 1 h with temperature of 50°C.
Cross section of the coated silicon and the front view of the coated PET film were imaged by field emission scanning electron microscopy (FESEM; Hitachi, S-4800, Tokyo, Japan). Contact angle measurement was conducted by the sessile drop technique on the surface of the PET films. Deionized water drop tests were carried out on each of the samples using 0.4-μl-size droplet on each testing. The wetting property level of Al2O3-coated PET film was measured by a static contact angle analysis system (JC2000A, Powereach, Shanghai, China). Atomic force microscopy (AFM; NanoScope IV SPM, Veeco, Plainview, NY, USA) was used to examine the surface morphology of the PET film before and after Al2O3 deposition using the tapping mode. Fourier transform infrared (FTIR) spectra of the films were measured using the Thermo Nicolet Nexus 670 (Thermo Scientific, Waltham, MA, USA), Smart iTR (diamond ATR, Thermo Scientific) with the spectral range of 650 to 4,000 cm−1 with the resolution of 4 cm−1. Chemical composition of Al2O3-coated PET film was evaluated by X-ray photoelectron spectroscopy (XPS).
Results and discussion
Surface morphology of the deposited Al2O3 film
It was shown that the cracks form above the aluminum oxide deposited on the PET films by plasma pretreated ALD and PA-ALD, during which the plasmas are responsible for not only the fragmentation of molecule precursors but also the detrimental effect on the aluminum oxide layers deposited on the PET surfaces. The energetic ion bombardment in the plasmas can create surface defect sites, which is considered to be the reason for the formation of cracks . On the other hand, the energetic ion bombardment reduces the activation energy for chemisorption and limits the formation of solid compound , which fills the requirement for the self-limiting deposition in ALD wherein the binding energy of a monolayer chemisorbed on the surface is higher than the binding energy of subsequent layers on top of the formed layer.
Furthermore, the uppermost polymer surface with the Ar plasma exposure may incorporate the oxygen by cross-linking reactions. It induces the presence of trace oxygen to react with the precursor molecules that lead to the occurrence of numerous peel-off sites . Although the cracks appear on the PET surface coated by ALD with plasma pretreatment and PA-ALD, the deposited surface area achieves the smooth state. It indicates that the necessary chemical functional groups induced due to the energetic ion bombardment in plasmas have a significant role on the initial growth on the PET surfaces.
Wettability of the deposited Al2O3 film
Figure 5 also shows the recovering of water contact angle as a function of time. It shows that the induced modifications on the wettability of the Al2O3 film on PET are not permanent since the contact angle increases to around 86° in about 2 days, which approaches that of the uncoated PET film. The recovering of water contact angle suggests the decrease of surface free energy with aging time , which is caused by the reorientation of induced polar chemical groups into the bulk of the material [18, 19]. It is also worth noting that the water contact angles of Al2O3 films deposited by ALD and plasma pretreated ALD (approximately 94°) are higher than that of PA-ALD (approximately 88°) after 3 days of aging. It can be attributed to the cracks formed on the deposited Al2O3 film, as shown in Figure 3, which also reduce the water contact angle.
The amplitude of the absorption peak at 3,429 cm−1 is found to be enhanced with the Al2O3 deposition by ALD, especially with the introduction of plasmas in ALD, which suggests the elevated density of -OH group on the surface of Al2O3 film deposited by PA-ALD. The -OH groups, acting as the reactive nucleation sites, are important to improve the quality of the deposited films in terms of uniformity and conformal film coverage without substantial subsurface growth .
Chemical composition of the deposited Al2O3 film
Figure 8a gives the XPS spectra of C 1s with the uncoated PET, which show the peaks of C1, C2, and C3, in the range of 284.77 to 284.80 eV, 285.47 to 286.32 eV, and 288.84 to 289.05 eV, corresponding to the -C-C- (and C-H bonds), the -C-O (and/or -C-OH), and the O=C-O (and/or COOH), respectively, which are consistent with the published data on PET film [25–27]. In Figure 8b with the Al2O3-coated PET films by PA-ALD, the spectra show another peak of C4 at 286.86 eV, corresponding to the -C-OH, besides the peaks of C1, C2, and C3, which indicates that a new chemical state is formed on the Al2O3-coated PET by PA-ALD. As shown in Figure 8c, the appearance of C4 is followed by the reduction of C2 peak amplitude significantly, which indicates the presence of -C-OH on the PET surfaces [25, 26]. The improvement on the formation of hydroxyl groups in PA-ALD is consistent with the FTIR results shown in Figure 6 that the highest amplitude of hydroxyl groups at the band of 3,429 cm−1 is also achieved by PA-ALD.
Figure 9a,b shows the O 1s peaks of uncoated PET and the Al2O3-coated PET film by PA-ALD. It shows that the spectrum of uncoated PET consists of O1 and O2 at the range of 531.43 to 532.16 eV and 533.64 eV, corresponding to the C=O and the C-O-, respectively . On the other hand, the spectrum of Al2O3-coated PET film by PA-ALD consists of O3 and O4 at the range of 532.16 to 532.54 eV and 530.72 to 530.81 eV, corresponding to the Al2O3 (and Al-O-C) and the O in AlO of AlOOH, respectively [25, 28]. It proposes the different deposition mechanism and dynamics during the ALD process. The detailed relative elemental contents of the uncoated PET and the Al2O3-coated PET films by ALD, plasma pretreated ALD, and PA-ALD are presented in Figure 9c. It shows that the Al2O3-coated PET films by ALD and plasma pretreated ALD consist of O1 and O3, which suggests that the element of C-O- is replaced by Al2O3 (and Al-O-C) during the ALD process. By introducing plasma in the ALD process, both the elements of C=O and C-O- are replaced by Al2O3 (and Al-O-C) and AlO in PA-ALD, which suggests the elimination of the CO-related elements and secures a normal growth of alumina oxide film on the PET film.
The successful deposition of Al2O3 film on PET is achieved by ALD, plasma pretreated ALD, and PA-ALD, which is demonstrated by surface morphology and chemical composition of the deposited Al2O3 film. The introduction of plasma in the ALD process is found to be crucial for the initial growth of ALD deposition by forming the chemical functional groups, such as hydroxyl -OH group, which is also mostly responsible for the enhancement of surface wettability in terms of water contact angle. Another issue concerning energetic ion bombardment has to be taken into account with the application of plasma, which induces the cracks on the deposited films. The characterization of chemical composition shows the formation of AlO element and elimination of CO-related elements in the Al2O3 film deposited by PA-ALD with plasma in the ALD process, which is different from that by ALD and plasma pretreated ALD and proposes a normal growth of Al2O3 on the polymer of PET in PA-ALD.
This work was supported by the Natural Science Foundation of China (grant no. 10835004 and 10905010) and sponsored by the Shanghai Shuguang Program (grant no. 08SG31) and the Fundamental Research Funds for the Central Universities.
- Ferguson JD, Weimer AW, Goerge SM: Atomic layer deposition of Al2O3 films on polyethylene particles. Chem Mater 2004, 16: 5602–5609. 10.1021/cm040008yView Article
- Cooper R, Upadhyaya HP, Minton TK, Berman MR, Du X, George SM: Protection of polymer from atomic-oxygen erosion using Al2O3 atomic layer deposition coatings. Thin Solid Films 2008, 516: 4036–4039. 10.1016/j.tsf.2007.07.150View Article
- Peng Q, Sun X-Y, Spagnola JC, Hyde GK, Spontak RJ, Parsons GN: Atomic layer deposition on electrospun polymer fibers as a direct route to Al2O3 microtubes with precise wall thickness control. Nano Letters 2007, 7: 719–722. 10.1021/nl062948iView Article
- Kääriäinen TO, Lehti S, Kääriäinen M-L, Cameron DC: Surface modification of polymers by plasma-assisted atomic layer deposition. Surf Coatings Techn 2011, 205: 475–479.View Article
- Beetstra R, Lafont U, Nijenhuis J, Kelder EM, van Ommen JR: Atmospheric pressure process for coating particles using atomic layer deposition. Chem Vapor Dep 2009, 15: 227–233. 10.1002/cvde.200906775View Article
- Puurunen RL: Surface chemistry of atomic layer deposition: a case study for the trimethylaluminum/water process. J Appl Phys 2005, 97: 121301. 10.1063/1.1940727View Article
- Kääriäinen TO, Cameron DC: Plasma-assisted atomic layer deposition of Al2O3 at room temperature. Plasma Proc Pol 2009, 6: S237. 10.1002/ppap.200930605View Article
- Niskanen A: Radical enhanced atomic layer deposition of metals and oxides. PhD thesis. : University of Helsinki, Department of Chemistry; 2006.
- Heil SBS: Plasma-assisted atomic layer deposition of metal oxides and nitrides. PhD thesis. : Technische Universiteit Eindhoven, Department of Applied Physics; 2008.
- Hirvikorpi T, Nissi MV, Nikkola J, Harlin A, Karppinen M: Thin Al2O3 barrier coatings onto temperature-sensitive packaging materials by atomic layer deposition. Surf Coatings Techn 2011, 205: 5088–5092. 10.1016/j.surfcoat.2011.05.017View Article
- Wilson CA, Grubbs RK, George SM: Nucleation and growth during Al2O3 atomic layer deposition on polymers. Chem Mater 2005, 17: 5625–5634. 10.1021/cm050704dView Article
- Kääriäinen TO, Maydannik P, Cameron DC, Lahtinen K, Johansson P, Kuusipalo J: Atomic layer deposition on polymer based flexible packaging materials: growth characteristics and diffusion barrier properties. Thin Solid Films 2010, 519: 3146–3154.View Article
- Kemell M, Färm E, Ritala M, Leskelä M: Surface modification of thermoplastics by atomic layer deposition of Al2O3 and TiO2thin films. Europ Pol J 2008, 44: 3564–3570. 10.1016/j.eurpolymj.2008.09.005View Article
- Rai VR, Vandalon V, Agarwal S: Surface reaction mechanisms during ozone and oxygen plasma assisted atomic layer deposition of aluminum oxide. Langmuir 2010, 26: 13732–13735. 10.1021/la101485aView Article
- Martin PM: Handbook of Deposition Technologies for Films and Coatings. Oxford: Elsevier; 2010.
- Morent R, Geyter ND, Verschuren J, Clerk KD, Kiekens P, Leys C: Non-thermal plasma treatment of textile. Surf Coatings Techn 2008, 202: 3427–3449. 10.1016/j.surfcoat.2007.12.027View Article
- Katsikogianni M, Amanatides E, Mataras D, Missirlis YF: Staphylococcus epidermis adhesion to He, He/O2 plasma treated PET films and aged materials: contributions of surface free energy and shear rate. Colloids Surf B Biointerfaces 2008, 65: 257–268. 10.1016/j.colsurfb.2008.04.017View Article
- Yang S, Gupta MC: Surface modification of polyethyleneterephthalate by an atmospheric-pressure plasma source. Surf Coatings Techn 2004, 187: 172–176. 10.1016/j.surfcoat.2004.03.057View Article
- Morent R, Geyter ND, Leys C, Gengembre L, Payen E: Study of the ageing behavior of polymer films treated with a dielectric barrier discharge in air, helium and argon at medium pressure. Surf Coatings Techn 2007, 201: 7847–78854. 10.1016/j.surfcoat.2007.03.018View Article
- Urbanová M, Šubrt J, Galíkova A, Pola J: IR laser ablative degradation of poly(ethylene terephthalate): formation of insoluble films with differently bonded C=O groups. Pol Degrad Stability 2006, 91: 2318–2323. 10.1016/j.polymdegradstab.2006.04.016View Article
- Djebara M, Stoquert JP, Abdesselem M, Muller D, Chami AC: FTIR analysis of polyethylene terephthalate irradiated by MeV He+. Nucl Instr Meth Phys Res 2012, 274: 70–77.View Article
- Nand AV, Ray S, Sejdic JT, Kilmartin PA: Characterization of polyethylene terephthalate/polyaniline blends as potential antioxidant materials. Mater Chem Phys 2012, 134: 443–450. 10.1016/j.matchemphys.2012.03.015View Article
- Awasthi K, Kulshrestha V, Avasthi DK, Vijay YK: Optical, chemical and structural modification of oxygen irradiated PET. Radiat Meas 2010, 45: 850–855. 10.1016/j.radmeas.2010.03.002View Article
- Hyde GK, Scarel G, Spagnola JC, Peng Q, Lee K, Gong B, Roberts KG, Roth KM, Hanson CA, Devive KC, Stewart AM, Hojo D, Na J-S, Jur JS, Parsons GN: Atomic layer deposition and abrupt wetting transition on nonwoven polypropylene and woven cotton fabrics. Langmuir 2010, 26: 2550–2558. 10.1021/la902830dView Article
- Ardelean H, Petit S, Laurens P, Marcus P, Khonsari FA: Effect of different laser and plasma treatments on the interface and adherence between evaporated aluminium and polyethylene terephthalate films: X-ray photoemission, and adhesion studies. Appl Surf Sci 2005, 243: 304–318. 10.1016/j.apsusc.2004.09.122View Article
- Cheng C, Liye Z, Zhan R-J: Surface modification of polymer fibre by the new atmospheric pressure cold plasma jet. Surf Coatings Techn 2006, 200: 6659–6665. 10.1016/j.surfcoat.2005.09.033View Article
- Vassallo E, Cremona A, Ghezzi F, Ricci D: Characterization by optical emission spectroscopy of an oxygen plasma used for improving PET wettability. Vacuum 2010, 84: 902–906. 10.1016/j.vacuum.2009.12.008View Article
- Crist BV: Handbook of Monochromatic XPS Spectra. California: XPS International; 2005.
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.